### van der Waals dispersion interactions in molecular

### materials: beyond pairwise additivity

Anthony M. Reillyaband Alexandre Tkatchenko*b

van der Waals (vdW) dispersion interactions are a key ingredient in the structure, stability, and response properties of many molecular materials and essential for us to be able to understand and design novel intricate molecular systems. Pairwise-additive models of vdW interactions are ubiquitous, but neglect their true quantum-mechanical many-body nature. In this perspective we focus on recent developments and applications of methods that can capture collective and many-body eﬀects in vdW interactions. Highlighting a number of recent studies in this area, we demonstrate both the need for and usefulness of explicit many-body treatments for obtaining qualitative and quantitative accuracy for modelling molecular materials, with applications presented for small-molecule dimers, supramolecular host–guest complexes, andﬁnally stability and polymorphism in molecular crystals.

### 1

### Introduction

The study of intermolecular or non-covalent interactions has
long been key to our understanding of complex molecular
systems, particularly when considering the assembly of
mole-cules into supramolecular systems or condensed matter.
Pre-dicting and studying cohesion in molecular materials relies
heavily on accurate and physically realistic treatments for the
diﬀerent intermolecular forces that arise in such materials, with
those that result from instantaneousuctuations of electrons,
which are referred to as dispersion or van der Waals (vdW)
interactions,† being particularly important. Although they are
typically weaker than electrostatic interactions or hydrogen
bonding, their long-ranged nature and ubiquity in all molecular
systems means they can always play an important role in
non-covalent binding.1,2_{Indeed, as they scale with system size, in}
some cases strongly non-linearly,3_{their importance can grow}
for larger molecules and molecular assemblies.

Dispersion interactions are quantum-mechanical in nature and form part of the correlation energy of a system. They stem from the inherent zero-point uctuations of electrons on an atom, which give rise to instantaneous multipole moments. These moments induce multipole moments on other atoms, which then interact with the original moment. The leading

order contribution is from dipole–dipole interactions, with a 1/
R6_{dependence on distance.}

The ability of an atom to form such moments (both
instan-taneous and induced) depends on its polarisability. The
polar-isability of an atom is inuenced by its chemical bonding but
also by its environment through polarisation and induction
eﬀects, where it is changed by coupling to the electric eld of its
surrounding atoms. Such eﬀects are known to be non-additive
in nature,1 _{and are important for going beyond simple point}
charges in the modelling of electrostatics in forceelds,4,5_{and}
modelling molecular polarisabilities.6

However, despite the central role of polarisability in vdW interactions, the vast majority of models ignore its non-additive and non-local nature, using simple pairwise-additive models with dispersion coeﬃcients that do not capture any dependence on non-local environment. In neglecting many-body eﬀects, these methods oen require empirical tting of parameters to a given molecule and environment.2,7

Pairwise-additive descriptions of vdW interactions have proven qualitatively successful in numerous applications ranging from bio-molecular simulations to modelling crystal-lisation. However, in recent years there has been a surge in interest in developing more sophisticated and quantitatively accurate approaches. The challenge of structure prediction,

including polymorphism in molecular crystals,8,9 _{and the}

availability of good-quality benchmark datasets10–12have driven developments for more realistic and less empirical approaches to vdW interactions.

Many of the developments in our understanding of vdW interactions in molecular systems have taken place in the context of vdW-inclusive density-functional theory (DFT). Workhorse semi-local and hybrid density functionals neglect long-range

correlation13 _{and considerable progress has been made in}

a

The Cambridge Crystallographic Data Centre, 12 Union Road, Cambridge, CB2 1EZ, UK

bFritz-Haber-Institut der Max-Planck-Gesellscha, Faradayweg 4-6, Berlin 14195,

Germany. E-mail: tkatchen@i-berlin.mpg.de; Tel: +49 3084134802

† In the chemistry community van der Waals interactions may refer to any non-covalent interaction, whereas in the (chemical-) physics community the terms dispersion and van der Waals interactions are largely synonymous and are used interchangeably, as we will do here.

Cite this:Chem. Sci., 2015, 6, 3289

Received 3rd February 2015 Accepted 29th March 2015 DOI: 10.1039/c5sc00410a www.rsc.org/chemicalscience

## Science

### PERSPECTIVE

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

Creative Commons Attribution 3.0 Unported Licence.

**View Article Online**

augmenting semi-local density functionals with non-local vdW
contributions.14–16 However, many of these vdW-inclusive DFT
approaches are still founded on pairwise models of dispersion
interactions, as use of fully ab initio approaches, such the
random-phase approximation,15_{is not feasible due to their far}
higher computational cost than standard semi-local DFT.

Despite their successful application in many areas, including
occasional successes for crystal-structure prediction,17_{}
quanti-tative and qualiquanti-tative failures remain when employing pairwise
models of vdW interactions.18–21_{As a result, in recent years there}
has been considerable interest in studying and modelling
non-additive and many-body contributions to vdW interactions,
which can take a number of forms.22_{In this perspective article}
we highlight collective eﬀects in vdW interactions in molecular
materials, focusing on non-additivity in polarisabilities and
methods that can capture these eﬀects, in particular, the
recently developed many-body dispersion (MBD) method.23,24
Using a number of applications, we illustrate new insights into
the role of collective vdW eﬀects in the stability and properties
of molecule materials. For a more in-depth discussion of the
theory and physics of many-body vdW interactions the reader is
referred to recent papers concerning a number of diﬀerent
approaches to the problem.15,24–27

In the following section (Section 2) we briey overview the theory of widely used pairwise descriptions of vdW interactions, before discussing the role of polarisation eﬀects in vdW inter-actions and introducing a number of approaches to many-body van der Waals in Section 3. We illustrate the application of these methods to diﬀerent systems in Section 4 before nally dis-cussing the prospects and challenges for understanding and modelling collective vdW interactions in Section 5.

### 2

### Pairwise-additive descriptions of

### van der Waals interactions

One of the most widespread pictures and models of vdW interactions is the pairwise-additive one, whereby the vdW energy of a collection of atoms or molecules can be expressed as

summation of attractive contributions from localised

multipoles: EvdW¼ XN ij;i . j C6ij Rij6 C8ij Rij8 C10ij Rij10 . ! (1) where Rijis the interatomic or fragment separation and C6ijis

dipole–dipole dispersion coeﬃcient for atoms or fragments i and j, with C8representing dipole–quadrupole and C10

repre-senting quadrupole–quadrupole and dipole–octupole disper-sion coeﬃcients. The disperdisper-sion coeﬃcients are determined by the corresponding polarisabilities of the atoms or fragments, relating the extent to which valence electrons can respond to local electric-eld uctuations. For the leading-order C6 term

the dispersion coeﬃcient can be expressed as1,28
C6ij¼_{p}3

ðN 0

aiðiuÞajðiuÞdu; (2)

where a(iu) is the frequency-dependent dipole polarisability.
Eqn (1) has its origin in second-order perturbation theory,
where the vdW interactions of two well-separated atoms can be
shown to have a 1/R6_{dependence. At small interatomic }

sepa-rations eqn (1) is clearly not physical, as the vdW energy

diverges to N. This arises from its derivation for

well-separated fragments at long ranges. As a practical solution, in nearly all applications of the pairwise model damping is required at short distances. The foundation of many

empirical force elds is the Lennard-Jones potential,7

ELJðRijÞ ¼

XN ij;isj

43 ðs=RijÞ12 ðs=RijÞ6

; where the parameter s
controls the balance between the attractive vdW term and a
short-range repulsion term, which models eﬀects such as Pauli
repulsion, or direct overlap of electron clouds. In vdW-inclusive
DFT, damping functions are commonly used to switch oﬀ the
vdW interaction at short distances,14,16 _{not only due to this}
divergence but also because widely employed density
func-tionals include short-range correlation, of which the vdW
energy forms a part. These damping functions oen contain
one or two functional-specic parameters, which may control
the distance at which the damping takes eﬀect,14,16_{or even scale}
some or all of the coeﬃcients to “match” better with DFT
energies.29,30

Within the pairwise description of van der Waals
interac-tions the accuracy obtainable (i.e. ignoring potential
non-addi-tive or high-order contributions) is governed by the dispersion
coeﬃcients used, whether to include higher than dipole
contributions, and the damping or short-range attenuation of
the interaction. Empirical potentials typically employ sets of
parameterstted to broad classes of molecules, e.g.
bio-mole-cules,31 _{organic molecules in a specic phase,}32,33 _{or small}
groups of molecules.34 _{The} _{tting of such potentials can be}
highly empirical, with diﬀerent terms in the potential
compensating for deciencies in other terms. Indeed,
trans-ferability of empirical potentials is a serious issue for this
reason.2

In vdW-inclusive DFT, early approaches employed empirical
parameter sets as well,29,35_{but more recent approaches aimed at}
more physically grounded schemes for obtaining dispersion
coeﬃcients, depending on hybridisation of atoms or the local
electron density.30,36,37_{This is the}rst type of collective eﬀect in
vdW interactions,22_{where crowding of an atom by its }
neigh-bours results in reduction of polarisabilities from ideal
free-atom values. The Tkatchenko–Scheﬄer (TS) model (also
referred to as the DFT + vdW approach) uses the local Hirshfeld
volume of an atom (Veﬀ) to reweigh accurate free-atom

polar-isabilities, C6 coeﬃcients, and van der Waals radii for this

eﬀect: Ceff 6ii ¼ Veff i Vfree i !2 Cfree 6ii : (3) Reff 0i ¼ Veff i Vfree i !1 3 Rfree 0i : (4)

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

aeffi ¼ Veff i Vfree i ! afreei : (5)

The resulting C6 coeﬃcients are functionals of the local

electron density and capture hybridisation eﬀects well, with an
accuracy of 5.5% for small molecules.36_{When used in DFT a}
damping function is required, with a single parametertted to
the functional employed. Given its small-molecule accuracy and
its ability to capture local eﬀects on vdW interactions, we will
use TS as a benchmark to illustrate the importance of
many-body and collective eﬀects. Other approaches, such as
atom-centred potentials38 _{and self-consistent vdW density }
func-tionals39 _{are also employed in DFT: the interested reader is}
referred to a number of reviews on vdW-inclusive DFT.14,16,40

For suﬃciently small or weakly polarisable systems, the
pairwise-additive approximation is of enormous use and can be
remarkably accurate. However, most molecular systems of
interest are neither small nor weakly polarisable. Furthermore,
in many instances it is diﬀerences in vdW energies that will
govern important phenomena such as polymorphism and
self-assembly, magnifying the importance of even small
contribu-tions. Such diﬀerences oen depend on comparing molecules
in very diﬀerent environments. For example, the lattice energy
of a molecular crystal is the balance between the energy of the
solid lattice and that of a single isolated molecule. The vast
diﬀerence in environments make collective eﬀects that depend
on an atom's or molecule's surroundings all the more
impor-tant. Pairwise-additive models of vdW interaction will generally
favour denser clusters and crystals, ignoring the contributions
of specic arrangements of atoms and molecules in a molecular
material. As such, pairwise-additive models can fail to model
molecular materials both quantitatively and qualitatively.
Quantitatively, ignoring collective eﬀects leads to many pairwise
methods overestimating cohesive energies of molecular
crys-tals19,41_{and host–guest systems,}21,42_{while also failing to capture}
the scaling of vdW interactions in diﬀerent nano-materials,
such as fullerenes.3,43 _{Qualitatively, many approaches fail to}
predict the correct polymorphic ordering of molecular crystals
of even relatively small molecules.18,20_{In the following section}
we will introduce a number of approaches to capturing
many-body or collective eﬀects in dispersion interactions. In Section 4
we will highlight the application of these methods to a number
of the examples given above, showing how collective models of
vdW interactions can overcome the limitations of pairwise
methods.

### 3

### Beyond pairwise-additive models

### for van der Waals interactions

Despite the widespread and oen successful application of pairwise-additive models of van der Waals interactions, it has long been known that they represent only an approximation to the true many-body nature of dispersion interactions. For this reason, a number of approaches have been developed to capture many-body contributions to vdW interactions, ranging from

simple three-body terms added to the pairwise expression to treatments that consider the collective nature of vdW correla-tions in a more fundamental manner.

3.1 Triple-dipole contributions

Given the origin of the pairwise approaches in second-order perturbation theory, the natural next step is to consider higher-order perturbative contributions. The Axilrod–Teller–Muto

(ATM) three-body term considers triple-dipole energy

contributions:1,44,45 EATM

Ri; Rj; Rk

¼C9ijkð3 cos qacos qbcos qcþ 1Þ

RijRjkRik3

; (6)

where the three angles qa, qband qcare the internal angles of the

triangle formed by the three atoms i, j and k, and C9ijkis the

triple-dipole coeﬃcient, which can also be obtained by
integra-tion of dipole polarisabilities over imaginary frequency,1_{but are}
also estimated from C6coeﬃcients.30Unlike the pairwise term,

the ATM expression can give both positive and negative
contri-butions depending on the triangle formed by the atoms,
although the major contribution is a repulsive one for an
equi-lateral triangle, which is a common occurrence in close-packed
solids.1,44_{The repulsion for an equilateral triangle arises because}
any interaction (e.g. formation of instantaneous and induced
dipoles) between any two atoms of the triangle is frustrated by
simultaneous interactions with the third, overall reducing the
interaction compared to three distinct pairs of atoms.

The application of the ATM term has varied in diﬀerent
elds, as therefore has the understanding of its role and
contribution. Its application to rare-gas solids yields a
qualita-tively correct picture of stability and elastic properties where
pairwise methods fail.46_{However, as evaluating eqn (6) for a}
collection of atoms necessitates a triple sum over the atoms, at
least in former times its used widespread use was prohibitively
expensive for force-eld simulations.7 _{In the} _{eld of }
vdW-inclusive DFT such costs are negligible compared to the
self-consistent cycle of the DFT calculation and a number of groups
have investigated their use.26,30,47 _{As we shall see below, the}
performance and importance of the ATM expression has been
mixed. Damping the ATM contribution and matching it with
pairwise contributions or a density functional are likely to be
part of the reason for this,26_{but it is also the case that the ATM}
expression is just therst in a series of perturbative many-body
contributions to vdW energy. Each of these terms can have
alternating signs and analytical expressions of higher-order

interactions become increasingly more cumbersome.1,48 _{A}

deeper understanding of collective vdW eﬀects requires going back to the denition of polarisability of molecules with many atoms, and this is what we do in the next section.

3.2 Non-additive eﬀects in the polarisability

To better understand how collective behaviour can aﬀect vdW interactions we need to step back and consider the denition of polarisability of molecular materials. The polarisability of a molecule or material relates the extent to which its electronic structure is distorted by an external electriceld. Specically,

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

the dipole polarisability,a relates an induced dipole moment to the applied electriceld:

m ¼ aE, (7)

wherem is the dipole moment of the atom and E is the local eld. The dipole polarisability is a 3 3 tensor by construction. Its non-local nature is critical to modelling polarisation and induc-tion eﬀects in molecular materials, which has been an active area of research and method development for many years.1,4,6,49,50 However, this aspect of polarisability and the importance of polarisation have largely been ignored in models of vdW actions, despite the central role of polarisability in such inter-actions [cf. eqn (2)]. Accurately modelling vdW interinter-actions requires considering polarisability and polarisation consistently. Such a collective model of polarisability and polarisation can be achieved using classical electrodynamics, where the inter-action between a collection of dipole polarisabilities can be modelled as:1,6,51 mp¼ ap Ep XN qsp Tpqmq ! ; (8)

wherempis the dipole moment of the pthatom,Epis the local

eld at p, and the term in brackets denotes the overall electric eld due to coupling with the dipole of the qth atom, through the dipole–dipole coupling tensor Tpq. Although this model is

classical, the input polarisabilities and denition of the coupling tensor can be based on a quantum-mechanical description. The coupling tensor is normally dened as:

Tij

pq¼ ViVjV(rpq), (9)

where i and j represent the Cartesian components of the vector joining p and q, and V is the Coulomb potential.

It is possible to rearrange this expression and cast it in a matrix form so that an eﬀective self-consistently screened (SCS) polarisability tensor can be dened that captures the eﬀect of coupling between all the dipoles:6,51

0 B B @ m1 m2 . mN 1 C C A ¼ 0 B B @ a11 T12 . T1N T21 a21 . T2N . . . . TN1 TN2 . aN1 1 C C A 10 B B @ E1 E2 . EN 1 C C A; 0 B B @ m1 m2 . mN 1 C C A ¼ B 0 B B @ E1 E2 . EN 1 C C A (10)

The eﬀective polarisability matrix, B, is oen referred to as
the relay matrix.6,51_{The eﬀective “screened” polarisability of e.g.}
the molecule or crystal, is obtained by fully contracting B.
Alternatively, the polarisability can be partitioned among the
atoms, with one practical scheme being to row or column
contract B:23

ap;SCS¼

XN q

Bpq; (11)

where Bpqis a 3 3 block of the 3N 3N relay matrix. The result

is an eﬀective polarisability for each atom or fragment, which even if the input polarisabilities are isotropic is in general anisotropic due to the environment of each atom. Some care must be taken in the denition of the Tpq, as the bare Coulomb

potential (1/|rq rp|) can lead to non-physical interactions

between atoms at short separations, where the distributed nature of the atomic dipoles must be properly accounted for.1 Damping of Tpq can yield reasonable results,6 but modelling

each dipole as having an isotropic Gaussian distribution
(cor-responding to an isotopic quantum harmonic dipole oscillator)
gives a simple but remarkably useful model.23,24,49 _{The above}
treatment can be performed using frequency-dependent
isabilities, leading to frequency-dependent screened
polar-isabilities and hence screened C6 coeﬃcients via eqn (2).23

Typically, this is done by rst obtaining the average of the
eigenvalues of the screened polarisability tensor for each atom.
As the TS polarisabilities are functionals of the local electron
density and already contain the important short-ranged eﬀect of
hybridisation,22,36_{they are an ideal choice for the input }
polar-isabilities in eqn (10), giving rise to the TS + SCS method for
obtaining screened polarisabilities and C6 coeﬃcients, which

can be used in a pairwise energy expression.

The screened polarisabilities and C6 coeﬃcients readily

illustrate deviations from the isotropic model of polarisability

and C6 oen used in force elds and vdW-inclusive DFT

methods. The polarisability tensor should be a positive
semi-denite 3 3 matrix, which can be represented by an ellipsoid,
in the same fashion as anisotropic displacement tensors are
depicted in crystallography.52_{Fig. 1 shows the screened }
polar-isability tensors of benzene and aspirin as ellipsoids. In
benzene, strong coupling in the plane of the molecule leads to
an increase of in-plane polarisability and a corresponding
reduction of out-of-plane polarisability. This is observed
exper-imentally in the molecular polarisability with the out-of-plane
polarisability being 55% of the in-plane value,6_{which is correctly}
captured by TS + SCS polarisabilities but not by the TS ones.25

For aspirin the same in-plane polarisation within its benzene ring can be observed, although now the diﬀerent groups surrounding the ring distort the polarisabilities to diﬀerent extents. Aspirin is a useful illustration of two competing polarisation eﬀects of electrodynamic screening. Within a molecule the eﬀect of collective vdW interactions on C6

coeﬃ-cients is to increase them, as atoms polarise strongly towards neighbours, with the average C6coeﬃcient of the C atoms in

aspirin being 43.3 a.u. compared to 31.0 a.u. for TS. However, in the solid state, coupling with the surrounding molecules limits an atom's ability to polarise with its neighbours, resulting in net depolarisation. This leads to an average C-atom C6of 39.0 a.u.

in aspirin, a reduction of around 10% relative to the gas phase.53
Comparing these coeﬃcients to values from condensed-phase
force elds is diﬃcult, as they typically involve balancing
dispersion, repulsion and electrostatic contributions and
frequently have very diﬀerent values. For example, an aromatic
C/C interaction in the W99 force eld has a dispersion
coef-cient of around 30 a.u.,33_{whereas in the UNI force}_{eld all}
C/C dispersion interactions have a coeﬃcient of 42 a.u.54

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

Fig. 2(a) shows the screened polarisability tensors of a “buckyball catcher” host–guest system (C60@C60H28).56The host

molecule exhibits dramatic departures from a model of spher-ical and near identspher-ical polarisabilities for each C atom. In some cases the polarisation is so strong and deviates so much from the isotropic model that the polarisability tensor is not positive semi-denite, although it is still possible to calculate C6

coef-cients for these atoms. Fig. 2(b) shows the change in TS + SCS C6coeﬃcients when the complex is formed. The blue spheres

denote atoms that depolarise when the complex is formed,

leading to a smaller C6 coeﬃcient. This depolarisation is

strongest at the interface between the two molecules and there is a clear asymmetry to the C60molecule. Using the TS + SCS C6

coeﬃcients in a pairwise expression for the dispersion energy
for this complex this yields a reduction of the binding energy of
the order of 30 kJ mol1 compared to TS,56 _{illustrating the}
importance of capturing these depolarisation eﬀects in
cohe-sion. The TS + SCS approach to pairwise vdW energies has been
applied to a number of systems by Buˇcko and co-workers,57_{and}
has shown that electrodynamic screening is important in a
variety of situations.

3.3 van der Waals correlations from the ACFD theorem

The self-consistently screened polarisabilities and C6

coeﬃ-cients discussed above capture important collective eﬀects in vdW interactions, as does the ATM expression for triple-dipole

contributions. However, the accurate treatment of vdW inter-actions requires methods than can capture both screening and many-body eﬀects in a systematic manner.22

Within the framework of the adiabatic connection
uctua-tion-dissipation (ACFD) theorem there is an exact expression for
the correlation energy in terms of density–density response
functions c(r,r0,iu), which describes the density response at r0as
a result of a perturbation at r.15 _{The correlation energy of a}
system can be written in terms of the response functions of a

corresponding mean-eld system (c0), and the response

Fig. 1 The anisotropic, screened polarisability tensors of (a) benzene and (b) aspirin. The tensors are represented as ellipsoids. Aliphatic H atoms are very strongly polarised towards their neighbouring C atom and are not shown for clarity.Mercury 3.4 has been used to produce theseﬁgures.55

Fig. 2 (a) The anisotropic, screened polarisability tensors of a “buckyball catcher” host–guest system and (b) a plot of the diﬀerence betweenC6coeﬃcients for the whole complex and the separate parts

(in the same geometry).56_{Some atoms polarise so strongly that they}

cannot be represented by an ellipsoid in (a). The size of the spheres in (b) indicates the magnitude of the diﬀerence, with blue meaning a decrease in C6 upon forming the complex and red denoting an

increase in the complex.

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

functions of a corresponding interacting system, where the Coulomb interaction v is scaled by a parameter l:58

Ec¼ 1 2p ðN 0 du ð1 0 dl Tr½clv c0v: (12)

The bare response function (c0) can be determined from the

eigenfunctions and eigenvalues of an electronic-structure

calculation,59 _{but some approximation is required for the}

interacting response functions. Within the popular random-phase approximation (RPA) the interacting response functions are approximated in terms of the non-interacting ones as follows:15,58 cRPA l ¼ c0 1 c0lv : (13)

RPA is commonly employed with DFT or HF orbitals and
contains the ring diagrams of coupled-cluster theory with
double excitations. RPA can have remarkable performance for
many properties in a variety of situations,15,60 _{particularly for}
long-range correlation and dispersion, but has a substantial
computational cost, scaling normally as N4or higher,61_{which}
has limited its widespread use. However, a recent N3algorithm
may increase its use.62

3.4 The many-body dispersion (MBD) method

The ACFD theorem gives a route to the correlation energy of a system in terms of response functions. While it is natural to consider the full response of a system based on a full and accurate representation of its electronic structure, model response functions could also be used to capture non-local correlation energy.

It is possible therefore to obtain an accurate but eﬃcient description of the long-range many-body van der Waals inter-actions by combining the ACFD expression for the correlation energy with response functions that model only the dipole response of an atom. This is the approach adopted by the

many-body dispersion (MBD) method,23 _{where the correlation or}

dispersion energy is given by:24 Ec;MBD¼ 1 2p ðN 0 duTr½lnð1 ATÞ; (14)

with T being an appropriate dipole–dipole coupling tensor and A is a diagonal 3N 3N matrix, with each block derived from an appropriate isotropic distributed polarisability: Alm¼ dlmal(iu).

In this expression the dipole response of each atom is modelled
using a single localised, isotropic quantum harmonic dipole
oscillator. The RPA treatment of this model considers all orders
of dipole coupling at long range, including triple and higher
dipole energies and collective screening simultaneously and
systematically.23,24,63 _{Due to the localised description of the}
response or polarisability, which is centred on atoms, the MBD
method is ideally suited to materials or systems with anite
band gap. The ACFD theorem expression can be recast as a
straightforward Hamiltonian expression,63_{which can then be}
directly diagonalised using simple and eﬃcient matrix algebra.

The contribution of the MBD energy to atomic forces is also straightforward to derive and implement.24

The MBD method has to-date largely been coupled with
density functional theory,23,64,65_{where the underlying functional}
accounts for short-range correlations. Therefore, some form of
range separation or damping of the MBD correlation energy is
required to avoid double counting, so that the MBD energy is
curtailed at short distances. This is reected in the input
polarisabilities and the denition of the dipole–dipole coupling
tensor. The polarisabilities are typically obtained in a two-step
process where short-range hybridisation eﬀects are considered
by using TS polarisabilities and screening contributions are

evaluated using the self-consistent screening equations

[eqn (8)]. More rigorous range separation can be achieved by considering only short-range screening contributions, as in the

MBD@rsSCS method,24 _{and in general this improves the}

performance of the method. A more in-depth discussion of the theory can be found in a number of recent publications.24,25

MBD has been combined with DFT largely due to the balance of accuracy and computational cost that this combination achieves, as we shall discuss below. However, MBD could be used to provide a model of long-range correlation or dispersion in other methods including empirical approaches such as force elds. Bereau and von Lilienfeld have recently introduced a scheme using MBD with polarisabilities derived from Voronoi tessellation.66

### 4

### Collective vdW interactions in

### dispersion coe

### ﬃcients, energies and

### response properties

Pairwise and collective models of vdW interactions have been applied in a wide variety of situations. Taking examples from small molecules, supramolecular systems and molecular crys-tals, in this section we highlight the importance of collective vdW methods in accurately modelling molecular materials. 4.1 Collective eﬀects in polarisabilities and dispersion coeﬃcients

We begin by briey discussing the role of collective eﬀects in polarisabilities and dispersion coeﬃcients of atoms and mole-cules in diﬀerent environments. For small molemole-cules, pairwise-additive methods can capture C6coeﬃcients quite well, with the

TS method has an accuracy of 5.5% for a set of 1225

small-molecule C6 values,67 and other pairwise methods and vdW

density functionals have values in the range of 8–30% using the
same or comparable test sets.30,68,69 _{However, the underlying}
polarisabilities of small molecules can still deviate substantially
from the isotropic model employed by pairwise-additive
approaches, as seen above for benzene and aspirin in Section
3.2. For 18 small molecules the TS method has a mean absolute
relative error of 76.3% for the fractional anisotropy of the
molecular polarisability with respect to experiment.25_{Including}
self-consistent screening, as in the TS + SCS method, captures a
substantial portion of this anisotropy, reducing the error to
33.5%.

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

In molecular crystals the role of collective eﬀects in mole-cules is more complex. As noted for aspirin above (Section 3.2), short-range polarisation within molecules increases C6

coeﬃ-cients while long-range depolarisation due to surrounding molecules decreases them. The acene crystals are an excellent example of this, with average C-atom C6coeﬃcient increasing

from naphthalene to pentacene for the isolated molecule but

decreasing in the solid as the molecule grows in size.70

Capturing these eﬀects is important for predicting the dielectric
constant and optical properties of the acene crystals. The TS
method overestimates dielectric constants substantially, while
TS + SCS is much closer to experiment and benchmark
calcu-lations.70,71_{Screened C}

6coeﬃcients of a set of semiconductors

obtained from time-dependent DFT (TDDFT) have also been shown to diﬀer signicantly from pairwise values, with a

pair-wise vdW term based on screened C6 coeﬃcients noticeably

improving the cohesive properties of the semiconductors.72_{The}
importance of defects and vacancies has also been studied in
semiconductors (using TS + SCS), showing that C6coeﬃcients

are signicantly altered by their presence, aﬀecting stability and defect migration barriers.73

Collective eﬀects in nanostructures lead not only to changes in C6 coeﬃcients but their fundamental scaling with system

size. For a pair of fullerenes pairwise-additive models predict a C6coeﬃcient between the two fullerenes that scales as n2, where

n is the number of C atoms in the fullerene. A number of recent
studies have shown larger power laws. TS + SCS gives scaling of
n2.35,3_{while modelling the polarisability using spherical shells}
of valence electron density yields a power law in the asymptotic
limit of n2.75.43_{TDDFT calculations of smaller fullerenes shows}
a power law of n2.2.74_{C}

6 coeﬃcients in other nanomaterials,

such as multilayer graphene and carbon nanotubes also feature
large and non-linear changes with system size that are not
captured by simple pairwise methods.3 _{This behaviour stems}
from the high symmetry and reduced dimensionality of these
systems (e.g.“0-D” fullerenes; “2-D” graphene), which lead to
very strong polarisation eﬀects. For layers of graphene sheets,
such eﬀects lead to stronger interactions within sheets, which
then reduces binding between sheets. TS overestimates the
binding between sheets substantially [87 meV per C atom versus
an experimental estimate of 52(2) meV per C atom]. In contrast,
PBE0 + MBD and RPA calculations agree much better with
experiment, with values of 50 meV per C atom and 48 meV per C
atom, respectively.24,75

While the role of non-additive behaviour in C6coeﬃcients is

minor in small molecules, it is clear that as we move to solids

and nanomaterials these eﬀects become much more

pronounced, changing not only absolute values but also altering fundamental scaling and behaviour. In the following subsec-tions we will discuss how this manifests itself in cohesive energies and properties.

4.2 Collective vdW interactions in molecular assemblies Isolated molecular assemblies, ranging from small molecular dimers to supramolecular host–guest complexes, are amongst some of the most widely used benchmarks used to evaluate and

understand vdW interactions and their contribution to
cohe-sion. For small molecular dimers there are a number of
data-bases of coupled-cluster singles, doubles and perturbative
triples [CCSD(T)] binding energies, representing a
“gold-stan-dard” benchmark with which to compare diﬀerent approaches.
The S22 and S66 databases of Hobza and co-workers contain
22 and 66 dimers,10,11 _{respectively, comprised of }
hydrogen-bonded interactions, vdW interactions and mixed bonding.

These databases have been used to assess pairwise C6/R6

methods,53,76 _{many-body dispersion (MBD)}24,53 _{and also vdW}

density functionals.77 _{In general, many pairwise methods}

perform well for these databases, yielding mean absolute errors
(MAEs) of 1–2 kJ mol1_{, better than the chemical-accuracy}

target of 4.2 kJ mol1. In comparison, semi-local functionals
without pairwise vdW contributions can yield errors greater
than 8 kJ mol1,76_{highlighting the importance of these }
inter-actions, even for simple systems. Considering collective vdW
contributions can further improve upon the performance of
pairwise methods,23,53_{but in general their role in these small}
systems is not dominant.

In larger supramolecular systems, collective eﬀects are clearly

more important. The S12L dataset of Grimme12 _{comprises 12}

supramolecular host–guest complexes. Risthaus and Grimme
found that including at least three-body vdW contributions
(from the ATM expression) was necessary for these systems, with
contributions of the order of 10 kJ mol1. The “buckyball
catcher” in Fig. 2 has a contribution of 13.4 kJ mol1_{from the}

ATM expression.21_{Three-body contributions generally improved}
pairwise methods, although not consistently, with D3 coupled to
the PBE functional78_{having a mean absolute error for binding}
energies of 8.8 kJ mol1but PBE + D3 + EATMhaving an MAE of

10 kJ mol1. The pairwise Tkatchenko–Scheﬄer vdW method

yields an MAE of the order of 30 kJ mol1,24 _{despite easily}
reaching chemical accuracy for small molecules. Including
collective vdW contributions using the MBD method reduces
this error dramatically to around 6.7 kJ mol1, approaching
close to the statistical error of benchmark diﬀusion Monte Carlo
binding energies for a subset of the S12L.42

Decomposition of the many-body contributions in the S12L
shows a signicant contribution from three-body interactions,
in line with the contribution seen with the ATM expression,21_{but}
the series only starts to converge with six-body contributions.42
These are not short-ranged interactions of the same nature as
the ATM-type three-body term, but rather the eﬀect on the
dispersion energy of coupling and polarisation of groups of six
atoms via more long-ranged 1/R3terms, as in eqn (10). In the
C60@C60H28system, even atoms in the C60molecule far from the

host molecule are aﬀected by screening, as can be seen from the change in C6coeﬃcients in Fig. 2(b). As the many-body

expan-sion typically alternates between positive and negative energy contributions, truncating at a lower order could lead to spurious over or under binding. Similar high-order contributions in DNA helices, where pairwise methods can omit more than 20% of the

full many-body vdW energy.79 _{Many-body contributions have}

also been found to be important for describing the conforma-tional preference of the Ac-Phe-Ala5-LysH+peptide chain.80It is

clear from these studies that modelling the binding of

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

supramolecular systems requires some model of collective and many-body vdW interactions.

4.3 Collective van der Waals eﬀects in molecular solids Molecular solids represent a diverse and challenging class of systems for applying diﬀerent descriptions of vdW interactions to diﬀerent properties, ranging from lattice energy to elastic properties and phonons.

4.3.1 Benzene crystal. Benzene is naturally one of the most widely studied molecular crystals. Recently, several groups have studied the lattice energy of benzene and have found it

important to include many-body contributions.47,81–84 One

approach is to expand the lattice energy as a mean-eld
contribution (e.g. a HF energy) plus a summation of
contribu-tions from dimers, trimers etc. within the lattice, calculated at a
high level of theory. As MP2 cannot capture three-body
disper-sion contributions, Kennedy et al. have been able to estimated
the three-body dispersion contribution by comparing MP2
energies for over 350 trimers from the crystal with CCSD(T)
energies and using the ATM expression for further more-distant
trimers.81_{The contribution is of the order of +3.2 kJ mol}1_{(i.e.}
reducing the magnitude of the lattice energy), around 6% of the
lattice energy, but smaller than previous estimates based solely

on the ATM expression with diﬀerent C9 coeﬃcients, which

range from 3.8–7.0 kJ mol1_{.}47,81,82

Yang et al. have used a similar expansion (including dimers,
trimers, tetramers and additional correlation contributions) to
estimate the benzene lattice energy as55.9(9) kJ mol1, which
compares very well with an experimental estimate of55.3(22)
kJ mol1obtained from sublimation enthalpies and theoretical
zero-point contributions.84 _{This value involved not only a}
signicant three-body contribution to the lattice energy but a

four-body one as well. It is worth noting that “body” is a

complete benzene molecule in these approaches, and thus these many-body contributions are not directly comparable to the three-atom contributions of the ATM expression.

The MBD method has also been applied to benzene, where the diﬀerence between the TS pairwise lattice energy and the

MBD lattice energy is around +11 kJ mol1 when both are

coupled to either the PBE or PBE0 (ref. 85) density functionals,
reducing the lattice energy to55.0 kJ mol1for PBE + MBD or
51.2 kJ mol1_{with PBE0 + MBD.}41_{The pairwise TS method,}
which is accurate to 1.5 kJ mol1for small-molecule binding
energies and 5.5% for C6 coeﬃcients,36,53 signicantly

over-estimates the lattice energy in the absence of collective screening and many-body energy contributions. The role of these eﬀects is even more pronounced when considering larger oligoacenes such as naphthalene and anthracene.41,70

4.3.2 X23 dataset. Recent eﬀorts to develop benchmark

dataset such as the C21 (ref. 19) and the X23 (ref. 41 and 53) have
permitted a broader assessment of absolute lattice energies with
various methods. The X23 is based on the C21 database and
contains a mixture of hydrogen-bonded solids, vdW-bound
solids and solids with a mixture of the two interactions.
Exper-imental lattice energies were determined from experExper-imental
sublimation enthalpies,86_{theoretical vibrational contributions}

(including vdW contributions) and, where available, experi-mental heat capacities, with an expected accuracy just better than chemical accuracy (4.2 kJ mol1), which is largely limited by experimental uncertainties in sublimation enthalpies.41

The TS pairwise method has a mean absolute error (MAE) for

the X23 of 10.0 kJ mol1 when coupled with the PBE0

func-tional, systematically overestimating lattice energies with an accuracy nearly an order of magnitude worse than that found for small dimers in the S22. Including many-body contributions with MBD yields an MAE of 3.9 kJ mol1, within the chemical-accuracy limit. The reduction in lattice energies is particularly pronounced for vdW-bound systems, as can be seen in Fig. 3, but is still important for hydrogen-bonded systems. The reduction in lattice energies arises from long-range depolar-isation of vdW interactions, as seen for C6coeﬃcients (Section

3.2) and repulsive many-body contributions, as would be partly obtained with the ATM expression (Section 3.1).

A number of other pairwise approaches have been tested
with the C21 and X23 databases, including XDM, D2 and
D3.19,41,87_{These methods have better MAEs than the TS pairwise}
approach, with D3 coupled with the TPSS meta-GGA
func-tional88_{being capable of reaching chemical accuracy as well.}

However, these methods typically have a more exible and

empirical approach to tting and determining the C6

coeﬃ-cients and damping of the short-range vdW interactions.19,29,76 For example, in the D2 approach there is a global and empirical scaling of C6coeﬃcients as part of the tting process for the

density functional employed. D3 and XDM both use the Becke–

Johnson damping function,89 _{which features an additional}

tting parameter compared to TS and does not damp the vdW
contribution to zero as R/ 0. The TS and MBD approaches are,
in part,tted to the S22 and S66 sets of small dimers to avoid
including eﬀects from larger molecules. D3 employs a wider set
of benchmark data,30_{while in XDM these parameters are oen}
re-tted for a specic basis set,90_{potentially factoring in other}
contributions into the parameters.

Fig. 3 The relative error in the calculate lattice energies for 22 vdW-bound and hydrogen-bonded systems. A positive value indicates overestimation of the experimental lattice energies; see ref. 41 for more details and a discussion on CO2.

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

Many of the empirical adjustments used in pairwise approaches would improve the performance of the TS method for molecular crystals, which we have noted before in the case of a global scaling of the TS C6coeﬃcients for solids.41However, such

adjustments limit the transferability of methods, creating
specic approaches for diﬀerent materials. As noted above,
Ris-thaus and Grimme advocate the use of the ATM expression in
host–guest systems. For molecular solids, using the ATM
expression has proven diﬃcult though. It requires an alternative
form of the XDM method's damping function, worsening the
underlying pairwise MAE and not yielding any additional
improvement.26_{For D3, the three-body contributions worsens the}
MAE for the TPSS functional by about 1.3 kJ mol1but improves
the HSE06 functional91_{result by 0.8 kJ mol}1_{.}87_{These }
inconsis-tent results with D3 and XDM methods stress the need for
methods that model vdW interactions seamlessly and
systemat-ically across a range of diﬀerent sizes and forms of molecular
materials. By including collective vdW eﬀects, MBD is able to
systematically improve upon the performance of the TS method,
providing an accurate method with minimal empiricism.

The non-local vdW-DF and vdW-DF2 functionals39,92_{have also}
been applied to the C21 set and show better performance than
TS but worse than MBD or XDM, with MAEs of 6.1 kJ mol1and
6.4 kJ mol1, respectively.19,41_{Such functionals model the }
long-range correlation by performing a double integral over the whole
electron density, summing contributions to the vdW using an
interaction kernel that has a 1/R6 dependence at long range.
Much of the work in improving these functionals has focussed
not on the non-local part but on the semi-local functional used
alongside it, as the performance of these methods is sensitive to
the coupling between the non-local correlation and the
semi-local functional used.14,92_{This can be exploited to tune these}
functionals to certain types of systems.93_{However, this leads to a}
broad spectrum of vdW-DF-based methods with their
perfor-mance wildly varying across a range of molecular materials.

4.3.3 Molecular-crystal polymorphism. The importance of

many-body contributions extends from lattice energies to
rela-tive lattice energies and the challenge of polymorphism, where
energy diﬀerences in the range of 0.1–1.0 kJ mol1_{need to be}

resolved.8,94_{On such scales even small many-body or collective}
vdW contributions can yield diﬀerent predictions for the most
stable polymorph or the low-energy portion of the polymorphic
landscape.

TS and MBD have been applied to a number of polymorphic systems, demonstrating the importance of collective eﬀects in these systems. Oxalic acid has two known forms, a and b [Fig. 4(a)]. Experimentally, the a form is found to be slightly

more stable by around 0.2 kJ mol1 in terms of lattice

energy.19,41,95 _{A number of pairwise vdW methods used in}

conjunction with DFT (including TS, XDM and D2)19_{}
systemat-ically overestimate the stability of the b form by up to 4 kJ mol1
[Fig. 4(b)]. Accounting for collective eﬀects using MBD and
employing the non-empirical hybrid functional PBE0 yields the
correct qualitative ordering. The D3 approach also yields the
correct ordering in conjunction with PBE0 but has a much
larger energy diﬀerence than observed experimentally,87_{while}
vdW-DF2 is also able to reproduce the correct ordering (note

however that this result will depend on the employed semi-local
approximation to the exchange–correlation functional).19 _{It is}
worth noting here that the best result in Fig. 4(b) in terms of
absolute diﬀerence (PBE + MBD) represents the wrong ordering
of the polymorphs. As methods oen aim to minimise MAEs it
is important that trends are still captured correctly. TPSS + D3
yields a smaller MAE for the X23 than PBE0 + D3 but incorrectly
predicts b oxalic acid to be more stable.87

Glycine is a challenging polymorphic system where
compu-tational methods oen have diﬃculties. An experimental
ordering has been established for three known polymorphs of
glycine, with the g one being be the most stable, followed by a
and then b. The TS pairwise method systematically
over-estimates the stability of the a and b forms, while again
including collective eﬀects the correct experimental ordering is
obtained with PBE0 + MBD.20_{The potential-energy surface and}
geometry of glycine is also markedly aﬀected by many-body
contributions.

Fig. 4 (a) The hydrogen-bonding interaction in a and b oxalic acid. (b) The relative energies between the polymorphs from experiment and as obtained with a number of diﬀerent DFT methods.

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

Finally, oxalyl dihydrazide is another system where many-body contributions have been explored, although only in the three-body ATM form. Two separate studies have shown the ATM expression aﬀecting relative energies by more than 1 kJ mol1,18which in one case leads to a diﬀerent ordering of the polymorphs.18,96The diﬀerence may arise in the damping of the three-body interaction or the manner in which the C9

coeﬃ-cients are determined.

The importance of collective vdW interactions in these systems is interesting, as they would normally be thought of as small hydrogen-bonded systems, where vdW interactions are very much a secondary concern. In larger systems the impor-tance of vdW interactions can grow and with it the role of collective vdW interactions. In Section 3.2 the signicant eﬀect of screening on the C6coeﬃcients of aspirin was highlighted.

Overall, the MBD lattice energy for form-I aspirin is reduced by
nearly 12 kJ mol1relative to the TS pairwise value.53_{Wen and}
Beran have estimated the 0 K lattice energy diﬀerence between
form-I and form-II aspirin to be of the order of0.1 kJ mol1
using MP2-based methods.97_{MBD agrees with this, yielding an}
essentially degenerate lattice energy diﬀerence for the two
forms. TS gives an energy diﬀerence of 0.2 kJ mol1_{in favour}

of form II (DE¼ EI EII). Despite the lattice energy change of

nearly 12 kJ mol1, the relative energies are very similar with the pairwise and many-body treatment. However, as we shall see below, going beyond the 0 K lattice energy reveals substantial diﬀerences between the two vdW treatments.

4.3.4 Beyond 0 K lattice energies. Many studies of poly-morphism focus on lattice potential energies, devoid of any zero-point or vibrational contributions. However, the nite-temperature stability of a given structure is dependent on lattice free-energy diﬀerences at a given temperature. In the harmonic limit these can be readily determined from phonon or solid-state vibrational spectra of the diﬀerent polymorphs.98,99

As noted above, the two known forms of aspirin100 _{are}

degenerate in terms of lattice energy when calculated with a
variety of diﬀerent methods. However, while intergrowth of the
two forms occurs,101_{form I appears to be the more }
thermody-namically stable and abundant form.102_{The free-energy }
diﬀer-ence between the two forms at 298 K is relatively small (0.7 kJ
mol1, favouring form II) when calculated with the TS pairwise
method. However, when the MBD method is used there is
signicant stabilisation of form I by 2.6 kJ mol1_{,}99_{rationalising}
experimental observations. This arises due to soening of
low-frequency vibrational modes in form I, making it entropically
stabilised. The diﬀerent arrangements of methyl groups and
hydrogen bonds in the lattice may explain the ability of
many-body interactions to inuence the vibrations diﬀerently in the
forms. Given the fact that the two forms are quite similar

structurally (diﬀering in weak C–H/O hydrogen bonds),100

such eﬀects are likely to be found in other polymorphic systems where more signicant diﬀerences can occur.

Dispersion interactions also play an important role in the
elastic or mechanical properties of molecular materials, which
are important for their processing and practical application, e.g.
tabletting of pharmaceuticals.103 _{Recently, the importance of}
pairwise vdW interactions has been highlighted for peptide

nanostructures.104_{Aspirin also highlights the role of collective}
vdW interactions in elastic behaviour. With the TS pairwise

method the bulk modulus of form-I aspirin is 12.40 GPa,99

compared to a value of 7.77 GPa at 300 K.105_{Collective vdW}
contributions reduce the calculated bulk modulus by over 20%
to 9.58 GPa, with a similar reduction for form II. Much of the
remaining diﬀerence is likely to arise from vibrational
contri-butions.106_{The shear modulus is also reduced by over 20% by}
many-body contributions in both forms. The reduction in the
strength of vdW interactions that arises to collective eﬀects is
more apparent in derived properties such as the elastic
constants. This phenomenon has also been seen using the TS +
SCS method, which has been used to determine the bulk
modulus of rare-gas molecular crystals by Buˇcko et al.57_{For }
rare-gas crystals the screened pairwise method reduces bulk moduli
by around 6–7%. For benzene, PBE with D2, TS, and TS + SCS all
yield a bulk modulus of 10 GPa,57,107,108 _{overestimating a 0 K}
experimental estimate of 8.0 GPa by 25%.109 _{In contrast, RPA}

based on PBE orbitals (Exx/RPA@PBE) yields a value of

7.5 GPa,110_{which is much closer to experiment.}

While the focus of research in vdW interactions has largely been on cohesive energies and structure, much of the importance of molecular materials derive from their properties. The study of elastic properties and vibrations already suggests that collective vdW eﬀects play an important role in governing the behaviour of molecular materials beyond their fundamental stability.

### 5

### Future directions and challenges

In recent years our understanding of the importance and role of van der Waals interactions, especially those of a collective nature, has substantially increased. Here, we highlight some of the diﬀerent aspects and areas of vdW interactions that still pose signicant challenges, while simultaneously oﬀering signicant opportunities for new insights.

Considerable eﬀort has been put into creating a number of
benchmark datasets for assessing diﬀerent approaches to
non-covalent interactions,10–12,19,41_{which have spurred development}
of new methods and our understanding of collective vdW
interactions. These have largely focused on energetics and to a
lesser extent geometry. For solids, obtaining suitable
bench-mark energies is challenging in the absence of a tractable
high-level computational method. Benchmark data for derived
properties, such as phonons and elastic properties, are even
harder to obtain from theory alone and experimental data
requires accounting for thermal and zero-point contributions.
However, further understanding of the importance of vdW
interactions hinges on new benchmark data to push and
chal-lenge computational methods. Gaining acceptance for new
general-purpose benchmark datasets, as the S22 and S66
already are for small-molecule dimers, is also crucial.

The role of many-body and collective vdW interactions in liquids and solutions, which play a critical role in so much of chemistry, has not been explored to the same extent as for solids or isolated systems. Probing such systems requires sampling of their dynamic behaviour, which is computationally demanding fromrst principles. However, as the recent work shows, it is

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

possible to decouple models of collective vdW interactions from
DFT, allowing their use in empirical potentials.66 _{The Drude}
oscillator model has been used to model induction and vdW
interactions in rare-gas liquids27_{and water.}111_{For general use,}
correlation between models of vdW interactions and e.g.

repulsion terms in force elds may make initial

parameter-isation and applications challenging. However, new forceelds
may lead to new insights into collective eﬀects on scales not
encountered in“perfect” molecular crystals or isolated
supra-molecular systems. For example, recent experimental work has
shown that the role of dispersion in molecular recognition of
apolar alkyl chains in solution appears to be much smaller than
anticipated from pairwise models of vdW interactions,112_{which}
might well stem from screening of vdW interactions.

Expanding the application of vdW-enabled methods will
require extending and developing these collective vdW methods
further. The MBD method at present considers only dipolar
responses to the vdW energy, ignoring higher multipole
contributions. While these contributions are short ranged
compared to the dipole term, which appears to be dominant in
many cases,41,113,114_{higher multipole contributions may well be}
more important for molecular materials at high pressures,
where atoms approach closer together. The model response
functions used in MBD could be extended to capture such
higher-order responses.24,25_{Currently, the use of MBD requires}
a single empiricallytted range-separation parameter to couple
it with a chosen density functional, just as pairwise methods
require one or more parameters in their damping functions.
Dening the range separation in terms of the functional itself or
developing new functionals implicitly alongside MBD would
remove this empiricism and may enhance its transferability.
Another area of on-going development is the application of
MBD to metallic systems. Due to its localised and atom-centred
nature, MBD is ideally suited to systems with a band gap.
Delocalised metallic states can lead to strong screening eﬀects
within the metal but also between surfaces and adsorbing
molecules, as captured by the vdWsurf_{method.}115_{MBD could be}
extended to capture these eﬀects by modelling delocalised
states alongside localised atom-centred contributions, with
Wannier functions being one possible route to achieve this.64

The importance of developing these methods and concepts further lies in the need to model, and ultimately design, hybrid materials that may contain diﬀerent manifestations of collec-tive vdW interactions. Such manifestations will need to be captured in a systematic and seamless manner to achieve this: an ongoing challenge for the vdW research community.

### 6

### Conclusions

Dispersion or vdW interactions are critical for the stability of

numerous molecular materials. However, many studies

consider such interactions only in a pairwise-additive form (mainly consisting of C6/R6terms), neglecting collective eﬀects

that originate from the quantum-mechanical many-body elec-tronic interactions they result from.

Considering these collective eﬀects in the dipole limit can yield screened polarisabilities and C6coeﬃcients for atoms that

can dramatically depend on the local and non-local environment of an atom or molecule, varying signicantly from “one size ts

all” C6 coeﬃcients used in many pairwise approaches. Such

environment-aware interactions could play an important role in
molecular recognition and assembly. Beyond capturing such
eﬀects in the coeﬃcients used in the pairwise expression, there
are additional many-body energy contributions that need to be
captured. The many-body dispersion method,23_{captures both}
eﬀects in an eﬃcient RPA-like treatment of dispersion and
non-local correlation, and has been used here to illustrate their role.
In small-molecule dimers collective eﬀects are not essential
for achieving accurate binding energies. However, in
supra-molecular systems even the simplest triple-dipole contribution
(from the ATM expression) can yield corrections to binding
energies of the order of 10 kJ mol1.21_{However, analysing the}
many-body energy suggests that contributions as high as sixth
order are needed for converged interaction energies, as the
collective eﬀect of atoms on polarisabilities is much more long
ranged than the three-body ATM energy contribution.

Many-body eﬀects are also important in molecular crystals. Recent work by a number of groups has highlighted the need for capturing three- and even four-molecule interactions to accu-rately model the stability of the comparatively “simple” and

symmetric benzene crystal.81,84 _{The MBD method corrects}

systematic overestimation of lattice energies found in the TS pairwise method and yields the correct polymorphic ordering for a number of challenging polymorphic systems. Adding three-body contributions to other approaches has yielded mixed results though, highlighting the need for methods that treat vdW interactions in a systematic and seamless manner.

More recent explorations of vdW interactions in response properties highlights the role of collective vdW interactions not just in stability but in the properties and function of molecular materials. More benchmark data are needed to fully explore these aspects of vdW interactions and there is also a need to move beyond static lattices and isolated systems to consider liquids, solutions, and disordered and dynamic systems.

### Acknowledgements

The authors acknowledge funding support from the European Research Council (ERC Starting Grant VDW-CMAT) and thank A. Ambrosetti, R. A. DiStasio Jr, V. V. Gobre, O. A. von Lilienfeld, N. Marom, M. Scheﬄer and G.-X. Zhang for numerous stimu-lating discussions and collaborations in thiseld.

### References

1 A. J. Stone, The Theory of Intermolecular Forces, Oxford University Press, UK, 2nd edn, 2013.

2 A. J. Stone, Science, 2008, 321, 787–789.

3 V. V. Gobre and A. Tkatchenko, Nat. Commun., 2013, 4, 2341.

4 P. Ren and J. W. Ponder, J. Comput. Chem., 2002, 23, 1497– 1506.

5 P. Ren, C. Wu and J. W. Ponder, J. Chem. Theory Comput., 2011, 7, 3143–3161.

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

6 B. T. Thole, Chem. Phys., 1981, 59, 341–350.

7 M. P. Allen and D. J. Tildesley, Computer Simulation of Liquids, Oxford University Press, Oxford, 1989.

8 S. L. Price, Acc. Chem. Res., 2009, 42, 117–126.

9 J. Bernstein, Polymorphism in Molecular Crystals, Oxford University Press, USA, 2007.

10 P. Jurˇecka, J. ˇSponer, J. ˇCern´y and P. Hobza, Phys. Chem. Chem. Phys., 2006, 8, 1985–1993.

11 J. ˇRez´aˇc, K. E. Riley and P. Hobza, J. Chem. Theory Comput., 2011, 7, 2427–2438.

12 S. Grimme, Chem.–Eur. J., 2012, 18, 9955–9964. 13 K. Burke, J. Chem. Phys., 2012, 136, 150901.

14 J. Klimeˇs and A. Michaelides, J. Chem. Phys., 2012, 137, 120901.

15 J. F. Dobson and T. Gould, J. Phys.: Condens. Matter, 2012, 24, 073201.

16 S. Grimme, Wiley Interdiscip. Rev.: Comput. Mol. Sci., 2011, 1, 211–228.

17 M. A. Neumann, F. J. J. Leusen and J. Kendrick, Angew. Chem., Int. Ed., 2008, 47, 2427–2430.

18 S. Wen and G. J. O. Beran, J. Chem. Theory Comput., 2012, 8, 2698–2705.

19 A. Otero-de-la-Roza and E. R. Johnson, J. Chem. Phys., 2012, 137, 054103.

20 N. Marom, R. A. DiStasio Jr, V. Atalla, S. Levchenko, A. M. Reilly, J. R. Chelikowsky, L. Leiserowitz and A. Tkatchenko, Angew. Chem., Int. Ed., 2013, 52, 6629–6632. 21 T. Risthaus and S. Grimme, J. Chem. Theory Comput., 2013,

9, 1580–1591.

22 J. F. Dobson, Int. J. Quantum Chem., 2014, 114, 1157–1161. 23 A. Tkatchenko, R. A. DiStasio Jr, R. Car and M. Scheﬄer,

Phys. Rev. Lett., 2012, 108, 236402.

24 A. Ambrosetti, A. M. Reilly, R. A. DiStasio Jr and A. Tkatchenko, J. Chem. Phys., 2014, 140, 18A508.

25 R. A. DiStasio Jr, V. V. Gobre and A. Tkatchenko, J. Phys.: Condens. Matter, 2014, 26, 213202.

26 A. Otero-de-la-Roza and E. R. Johnson, J. Chem. Phys., 2013, 138, 054103.

27 A. P. Jones, J. Crain, V. P. Sokhan, T. W. Whiteld and G. J. Martyna, Phys. Rev. B: Condens. Matter Mater. Phys., 2013, 87, 144103.

28 H. B. G. Casimir and D. Polder, Phys. Rev., 1948, 73, 360– 372.

29 S. Grimme, J. Comput. Chem., 2006, 27, 1787–1799. 30 S. Grimme, J. Antony, S. Ehrlich and H. Krieg, J. Chem.

Phys., 2010, 132, 154104.

31 C. Oostenbrink, A. Villa, A. E. Mark and W. F. Van Gunsteren, J. Comput. Chem., 2004, 25, 1656–1676. 32 W. L. Jorgensen, D. S. Maxwell and J. Tirado-Rives, J. Am.

Chem. Soc., 1996, 118, 11225–11236.

33 D. E. Williams, J. Comput. Chem., 2001, 22, 1154–1166. 34 D. C. Sorescu, B. M. Rice and D. L. Thompson, J. Phys.

Chem. B, 2000, 104, 8406–8419.

35 M. A. Neumann and M.-A. Perrin, J. Phys. Chem. B, 2005, 109, 15531–15541.

36 A. Tkatchenko and M. Scheﬄer, Phys. Rev. Lett., 2009, 102, 073005.

37 A. D. Becke and E. R. Johnson, J. Chem. Phys., 2007, 127, 154108.

38 O. A. von Lilienfeld, I. Tavernelli, U. Rothlisberger and D. Sebastiani, Phys. Rev. Lett., 2004, 93, 153004.

39 M. Dion, H. Rydberg, E. Schr¨oder, D. C. Langreth and

B. I. Lundqvist, Phys. Rev. Lett., 2004, 92, 246401.

40 A. Tkatchenko, L. Romaner, O. T. Hofmann, E. Zojer, C. Ambrosch-Draxl and M. Scheﬄer, MRS Bull., 2010, 35, 435–442.

41 A. M. Reilly and A. Tkatchenko, J. Chem. Phys., 2013, 139, 024705.

42 A. Ambrosetti, D. Alf´e, R. A. DiStasio and A. Tkatchenko, J. Phys. Chem. Lett., 2014, 5, 849–855.

43 A. Ruzsinszky, J. P. Perdew, J. Tao, G. I. Csonka and J. M. Pitarke, Phys. Rev. Lett., 2012, 109, 233203.

44 B. M. Axilrod and E. Teller, J. Chem. Phys., 1943, 11, 299– 300.

45 Y. Muto, Proc. Phys.-Math. Soc. Jpn., 1943, 17, 629–631. 46 G. J. Keeler and D. N. Batchelder, J. Phys. C: Solid State Phys.,

1970, 3, 510.

47 O. A. von Lilienfeld and A. Tkatchenko, J. Chem. Phys., 2010, 132, 234109.

48 W. L. Bade, J. Chem. Phys., 1958, 28, 282–284.

49 A. Mayer, Phys. Rev. B: Condens. Matter Mater. Phys., 2007, 75, 045407.

50 M. W. Cole, D. Velegol, H.-Y. Kim and A. A. Lucas, Mol. Simul., 2009, 35, 849–866.

51 J. Applequist, J. R. Carl and K.-K. Fung, J. Am. Chem. Soc., 1972, 94, 2952–2960.

52 K. N. Trueblood, H.-B. B¨urgi, H. Burzlaﬀ, J. D. Dunitz, C. M. Gramaccioli, H. H. Schulz, U. Shmueli and

S. C. Abrahams, Acta Crystallogr., Sect. A: Found.

Crystallogr., 1996, 52, 770–781.

53 A. M. Reilly and A. Tkatchenko, J. Phys. Chem. Lett., 2013, 4, 1028–1033.

54 A. Gavezzotti and G. Filippini, J. Phys. Chem., 1994, 98, 4831–4837.

55 C. F. Macrae, I. J. Bruno, J. A. Chisholm, P. R. Edgington, P. McCabe, E. Pidcock, L. Rodriguez-Monge, R. Taylor, J. van de Streek and P. A. Wood, J. Appl. Crystallogr., 2008, 41, 466–470.

56 A. Tkatchenko, D. Alf´e and K. S. Kim, J. Chem. Theory Comput., 2012, 8, 4317–4322.

57 T. Buˇcko, S. Leb`egue, J. Hafner and J. G. ´Angy´an, Phys. Rev. B: Condens. Matter Mater. Phys., 2013, 87, 064110.

58 H.-V. Nguyen and S. de Gironcoli, Phys. Rev. B: Condens. Matter Mater. Phys., 2009, 79, 205114.

59 (a) S. L. Adler, Phys. Rev., 1962, 126, 413–420; (b) N. Wiser, Phys. Rev., 1963, 129, 62–69.

60 X. Ren, P. Rinke, C. Joas and M. Scheﬄer, J. Mater. Sci., 2012, 47, 7447–7471.

61 X. Ren, P. Rinke, V. Blum, J. Wieferink, A. Tkatchenko, A. Sanlippo, K. Reuter and M. Scheﬄer, New J. Phys., 2012, 14, 053020.

62 M. Kaltak, J. Klimeˇs and G. Kresse, Phys. Rev. B: Condens. Matter Mater. Phys., 2014, 90, 054115.

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a

63 A. Tkatchenko, A. Ambrosetti and R. A. DiStasio Jr, J. Chem. Phys., 2013, 138, 074106.

64 P. L. Silvestrelli, J. Chem. Phys., 2013, 139, 054106. 65 M. Modrzejewski, G. Chalasinski and M. M. Szczesniak, J.

Chem. Theory Comput., 2014, 10, 4297–4306.

66 T. Bereau and O. A. von Lilienfeld, J. Chem. Phys., 2014, 141, 034101.

67 A. Tkatchenko and O. A. von Lilienfeld, Phys. Rev. B: Condens. Matter Mater. Phys., 2008, 78, 045116.

68 E. R. Johnson and A. D. Becke, J. Chem. Phys., 2005, 123, 024101.

69 O. A. Vydrov and T. Van Voorhis, Phys. Rev. A, 2010, 81, 062708.

70 B. Schatschneider, J.-J. Liang, A. M. Reilly, N. Marom, G.-X. Zhang and A. Tkatchenko, Phys. Rev. B: Condens. Matter Mater. Phys., 2013, 87, 060104.

71 S. Sharifzadeh, A. Biller, L. Kronik and J. B. Neaton, Phys. Rev. B: Condens. Matter Mater. Phys., 2012, 85, 125307. 72 G.-X. Zhang, A. Tkatchenko, J. Paier, H. Appel and

M. Scheﬄer, Phys. Rev. Lett., 2011, 107, 245501.

73 W. Gao and A. Tkatchenko, Phys. Rev. Lett., 2013, 111, 045501.

74 J. Kauczor, P. Norman and W. A. Saidi, J. Chem. Phys., 2013, 138, 114107.

75 S. Leb`egue, J. Harl, T. Gould, J. G. ´Angy´an, G. Kresse and J. F. Dobson, Phys. Rev. Lett., 2010, 105, 196401.

76 L. Goerigk, H. Kruse and S. Grimme, ChemPhysChem, 2011, 12, 3421–3433.

77 O. A. Vydrov and T. Van Voorhis, J. Chem. Phys., 2010, 133, 244103.

78 J. P. Perdew, K. Burke and M. Ernzerhof, Phys. Rev. Lett., 1996, 77, 3865–3868.

79 R. A. DiStasio Jr, O. A. von Lilienfeld and A. Tkatchenko, Proc. Natl. Acad. Sci. U. S. A., 2012, 109, 14791–14795. 80 M. Rossi, S. Chutia, M. Scheﬄer and V. Blum, J. Phys. Chem.

A, 2014, 118, 7349–7359.

81 M. R. Kennedy, A. R. McDonald, A. E. DePrince, M. S. Marshall, R. Podeszwa and C. D. Sherrill, J. Chem. Phys., 2014, 140, 121104.

82 S. Wen and G. J. O. Beran, J. Chem. Theory Comput., 2011, 7, 3733–3742.

83 R. Podeszwa, B. M. Rice and K. Szalewicz, Phys. Rev. Lett., 2008, 101, 115503.

84 J. Yang, W. Hu, D. Usvyat, D. Matthews, M. Sch¨utz and G. K.-L. Chan, Science, 2014, 345, 640–643.

85 C. Adamo and V. Barone, J. Chem. Phys., 1999, 110, 6158– 6170.

86 NIST WebBook and references within, http://

webbook.nist.gov/chemistry/name-ser.html, Accessed

September, 2014.

87 J. Moellmann and S. Grimme, J. Phys. Chem. C, 2014, 118, 7615–7621.

88 J. Tao, J. P. Perdew, V. N. Staroverov and G. E. Scuseria, Phys. Rev. Lett., 2003, 91, 146401.

89 E. R. Johnson and A. D. Becke, J. Chem. Phys., 2006, 124, 174104.

90 A. Otero-de-la-Roza and E. R. Johnson, J. Chem. Phys., 2012, 136, 174109.

91 (a) J. Heyd, G. E. Scuseria and M. Ernzerhof, J. Chem. Phys., 2003, 118, 8207–8215; (b) J. Heyd, G. E. Scuseria and M. Ernzerhof, J. Chem. Phys., 2006, 124, 219906.

92 K. Lee, E. D. Murray, L. Kong, B. I. Lundqvist and D. C. Langreth, Phys. Rev. B: Condens. Matter Mater. Phys., 2010, 82, 081101.

93 J. Klimeˇs, D. R. Bowler and A. Michaelides, J. Phys.: Condens. Matter, 2010, 22, 022201.

94 S. L. Price, Acta Crystallogr., Sect. B: Struct. Sci., Cryst. Eng. Mater., 2013, 69, 313–328.

95 H. G. M. de Wit, J. A. Bouwstra, J. G. Blok and C. G. de Kruif, J. Chem. Phys., 1983, 78, 1470–1475.

96 D. Presti, A. Pedone, M. C. Menziani, B. Civalleri and L. Maschio, CrystEngComm, 2014, 16, 102–109.

97 (a) S. Wen and G. J. O. Beran, Cryst. Growth Des., 2012, 12, 2169–2172; (b) Y. Huang, Y. Shao and G. J. O. Beran, J. Chem. Phys., 2013, 138, 224112.

98 S. Baroni, S. de Gironcoli, A. Dal Corso and P. Giannozzi, Rev. Mod. Phys., 2001, 73, 515–562.

99 A. M. Reilly and A. Tkatchenko, Phys. Rev. Lett., 2014, 113, 055701.

100 A. D. Bond, R. Boese and G. R. Desiraju, Angew. Chem., Int. Ed., 2007, 46, 615–617.

101 A. D. Bond, R. Boese and G. R. Desiraju, Angew. Chem., Int. Ed., 2007, 46, 618–622.

102 S. Varughese, M. S. R. N. Kiran, K. A. Solanko, A. D. Bond, U. Ramamurty and G. R. Desiraju, Chem. Sci., 2011, 2, 2236–2242.

103 S. Karki, T. Friˇsˇci´c, L. F´abi´an, P. R. Laity, G. M. Day and W. Jones, Adv. Mater., 2009, 21, 3905–3909.

104 I. Azuri, L. Adler-Abramovich, E. Gazit, O. Hod and L. Kronik, J. Am. Chem. Soc., 2014, 136, 963–969.

105 J. D. Bauer, E. Hauss¨uhl, B. Winkler, D. Arbeck, V. Milman and S. Robertson, Cryst. Growth Des., 2010, 10, 3132–3140. 106 Y. P. Varshni, Phys. Rev. B: Solid State, 1970, 2, 3952–3958. 107 T. Buˇcko, J. Hafner, S. Leb`egue and J. G. ´Angy´an, J. Phys.

Chem. A, 2010, 114, 11814–11824.

108 W. A. Al-Saidi, V. K. Voora and K. D. Jordan, J. Chem. Theory Comput., 2012, 8, 1503–1513.

109 E. J. Meijer and M. Sprik, J. Chem. Phys., 1996, 105, 8684– 8689.

110 D. Lu, Y. Li, D. Rocca and G. Galli, Phys. Rev. Lett., 2009, 102, 206411.

111 A. Jones, F. Cipcigan, V. P. Sokhan, J. Crain and G. J. Martyna, Phys. Rev. Lett., 2013, 110, 227801.

112 L. Yang, C. Adam, G. S. Nichol and S. L. Cockro, Nat. Chem., 2013, 5, 1006–1010.

113 N. Marom, A. Tkatchenko, M. Rossi, V. V. Gobre, O. Hod, M. Scheﬄer and L. Kronik, J. Chem. Theory Comput., 2011, 7, 3944–3951.

114 S. N. Steinmann and C. Corminboeuf, J. Chem. Theory Comput., 2012, 8, 4305–4316.

115 V. G. Ruiz, W. Liu, E. Zojer, M. Scheﬄer and A. Tkatchenko, Phys. Rev. Lett., 2012, 108, 146103.

Open Access Article. Published on 30 March 2015. Downloaded on 26/02/2016 10:27:53.

This article is licensed under a